Acta Materialia 55 (2007) 4475–4487 www.elsevier.com/locate/actamat Theory-guided bottom-up design of b-titanium alloys as biomaterials based on ﬁrst principles calculations: Theory and experiments ´ D. Raabe *, B. Sander, M. Friak, D. Ma, J. Neugebauer Max-Planck-Institut fur Eisenforschung, Max-Planck-Str. 1, 40237 Dusseldorf, Germany ¨ ¨ Received 17 March 2007; received in revised form 10 April 2007; accepted 12 April 2007 Available online 1 June 2007Abstract In this study we present a new strategy for the theory-guided bottom up design of b-Ti alloys for biomedical applications using aquantum mechanical approach in conjunction with experiments. Parameter-free density functional theory calculations are used to pro-vide theoretical guidance in selecting and optimizing Ti-based alloys with respect to three constraints: (i) the use of non-toxic alloy ele-ments; (ii) the stabilization of the body centered cubic b-phase at room temperature; (iii) the reduction of the elastic stiﬀness compared toexisting Ti-based alloys. Following the theoretical predictions, the alloys of interest are cast and characterized with respect to their crys-tallographic structure, microstructure, texture, and elastic stiﬀness. Due to the complexity of the ab initio calculations, the simulationshave been focused on a set of binary systems of Ti with two diﬀerent high melting body-centered cubic metals, namely, Nb and Mo.Various levels of model approximations to describe mechanical and thermodynamic properties are tested and critically evaluated.The experiments are conducted both, on some of the binary alloys and on two more complex engineering alloy variants, namely, Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta and Ti–20 wt.% Mo–7 wt.% Zr–5 wt.% Ta.Ó 2007 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.Keywords: Ab initio; Metallurgy; Quantum mechanics; Materials design; Bcc1. Introduction Commonly, Ti and Ti-base alloys occur in one or a mix- ture of two basic crystalline structures: the a-phase and the1.1. Engineering motivation for the development of b-phase, which assume a hexagonal (hex) and a body-cen-b-titanium alloys for biomaterials applications tered cubic (bcc) structure, respectively. Thus, three general classes of Ti-base alloys are deﬁned: a, a–b and b [1–30]. The design of novel Ti-based alloys for biomedical The transition temperature from the a- to the b-phase isload-bearing implant applications, such as hip or knee about 882 °C for pure Ti. Elements which promote higherprostheses, aims at providing structural materials which or lower transformation temperatures are referred to as aare characterized by a good corrosion stability in the stabilizers (like O, Al, La) or b stabilizers (like Mo, Nb,human body, high fatigue resistance, high strength-to- Ta), respectively.weight ratio, good ductility, low elastic modulus, excellent Recent studies have revealed that a compromise alongwear resistance, low cytotoxicity and a negligible tendency the biomedical constraints mentioned above can beto provoke allergic reactions [1–12]. obtained by designing Ti alloys which use the most bio- compatible elements, i.e. Ta, Mo, Nb and Zr, as alloy ingredients for stabilizing the bcc b-phase [6–26]. Experi- * Corresponding author. mental investigations on such alloy variants have shown E-mail address: email@example.com (D. Raabe). that these materials can indeed match most of the desired1359-6454/$30.00 Ó 2007 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.doi:10.1016/j.actamat.2007.04.024
4476 D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487properties outlined above, i.e. they do not reveal any toxic- 1.2. Motivation for applying ab initio calculations to theity vs. osteoblastic cells, have a high corrosion resistance, understanding and design of beta-titanium alloysand show good mechanical properties owing to solidsolution and particle strengthening while preserving the Owing to the arguments outlined above, the aim of thelight weight character of Ti. present study is to understand and design biocompatible An attractive feature of b Ti alloys is their low elastic b-phase Ti alloys with a small elastic modulus. However,modulus, which is below that of the conventional a or in contrast to earlier approaches, which used phenomeno-a–b Ti alloys commonly used for biomedical applications. logical rules in conjunction with metallurgical experienceThis latter property is of particular relevance because an for estimating a beneﬁcial alloy composition, we pursueimportant requirement of bone-replacing implants is a in this work a theory-guided bottom-up design strategylow elastic stiﬀness approximating as far as possible that to achieve that goal. The approach is based on the combi-of the surrounding bone tissue [13–25]. The background nation of ab initio simulations with experiments. The ab ini-of this aspect is the stress shielding eﬀect: bone is a living tio predictions are based on density functional theorymaterial which is subject to mechanical loads resulting (DFT) [31,32] in the generalized gradient approximationfrom the weight it carries and the motion it creates. When (GGA-PBE96) . They are used to provide theoreticalan elastically much stiﬀer surgical implant part replaces a guidance in selecting suited Ti-based alloys with respectportion of the human skeleton, it takes over a consider- to the three constraints of ﬁrst, using exclusively non-toxicable part of that mechanical load, thereby shielding the alloy elements; second, obtaining a stable body centeredremaining bone that surrounds and abuts the implant. cubic b-phase; and third, reducing the elastic stiﬀness.Reducing the physiological loads on the bone entails Following the theoretical predictions, the alloys of inter-resorption mechanisms which lead to a drop in bone den- est have been cast and characterized with respect to theirsity, mineralization state, strength and health. The structure, crystallographic texture and elastic stiﬀness.mechanical system bone–implant undergoes three main Since the ab initio simulations are applied to elucidate basiceﬀects upon stress shielding: ﬁrst, osteoporosis associated tendencies of suited alloy compositions under the con-with underutilization that characterizes tissue resorption straints described on the one hand and to optimize the the-subsequent to the absence or the decrease in local physio- oretical framework for such tasks on the other, they arelogical mechanical stress. Second, tissue resorption conﬁned in the ﬁrst step to a set of binary systems of Tiincreases the danger of formation and migration of wear with diﬀerent high melting bcc refractory transition metals,debris at the bone–implant interface via biological ﬂuid namely, Nb and Mo. The experiments are conducted bothtransport. Third, the stiﬀness gap between bone and mate- on some of the binary alloys and also on two more complexrial gives rise to micro-motions at the bone–implant engineering alloy variants, namely, Ti–35 wt.% Nb–7 wt.%interface. Zr–5 wt.% Ta and Ti–20 wt.% Mo–7 wt.% Zr–5 wt.% Ta. Owing to this context, the stress shielding and the The reasoning behind the use of ab initio calculationsdescribed eﬀects associated with it create multiple unde- for understanding and designing novel b-Ti alloys pursuessired phenomena at the bone–implant system and may the following strategy. First, we hope that a more system-ﬁnally lead to contact loosening, premature implant failure atic theoretical inspection of the structure and thermody-or debris-induced infections [27–30]. namics of such alloys provides a basic insight into the This phenomenon explains that in the design of Ti alloys electronic tendencies as a function of compositions whichfor biomedical applications the reduction of the elastic stiﬀ- provide a more detailed guideline to future alloy designness must be regarded as a high priority constraint in the approaches than commonly applied in the ﬁeld of metallur-overall strategy [6–26]. The major challenge associated with gical alloy design. Second, we aim at replacing empiricalthis point is documented by the fact that commercial pure rules for alloy design by rules which are built on the natureTi and a–b type Ti–6 wt.% Al–4 wt.% V alloys, which are of the electronic bond. Third, we hope to reduce the hugecurrently widely used as structural biomaterials for the eﬀorts commonly associated with experimental alloyreplacement of hard tissues in artiﬁcial joints, have an elas- screening in that ﬁeld (melting, casting, heat treatment,tic modulus of 105–110 GPa while human cortical bone has homogenization, thermodynamic and mechanical charac-a stiﬀness of about 20 GPa. terization) by using theoretical predictions of structure New alloys which are dominated by a large amount of and elastic properties. Fourth, a better understanding ofstable b-phase reveal a signiﬁcant drop in the elastic mod- alloy design on the basis of ab initio simulations can revealulus to values as small as 65 GPa [16–24]. It is, therefore, shortcuts to arriving at advanced promising alloy conceptslikely that the next generation of structural materials for as opposed to conventional metallurgical try and errorreplacing hard human tissue will be of this type. Another methods. Fifth, it is our aim to develop and critically eval-reason to develop a new generation of alloys is that con- uate the applicability of ab initio predictions in the ﬁeld ofventional two phase a–b variants such as Ti–6 wt.% Al– metallurgy by comparing the simulation results with exper-4 wt.% V contain both vanadium, a cytotoxic element, iments. Sixth, we want to prove that ab initio methods canand aluminum, an element suspected of causing neurolog- not only be of great service to investigating the stability ofical disorders. certain single crystalline structures but can also predict
D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487 4477mechanical properties which are of immediate engineering account only volume relaxation. The cell shape for therelevance for the ﬁnal product design. Seventh, we want to hcp phase was ﬁxed by keeping the c/a ratio constant toshow that in some cases – like in the present case of the the value of pure hcp Ti (c/a = 1.59).design of b-Ti alloys – a scale-jumping modeling strategy The fundamental quantity expressing the thermody-which directly predicts intrinsic properties, such as struc- namic stability of an alloy is the alloy formation energy.ture and elasticity, without the use of mesoscale methods The formation energy (per atom) of a Ti-binary alloycan for certain technological problems be more rewarding TixX1Àx (X = Nb, Mo here) in conﬁguration r = bcc/hcpand eﬃcient than multiscale modeling approaches which is deﬁned as:aim to combine predictions from many additional interme-diate scales for the same aim. Er ðTix X1Àx Þ ¼ Etot ðTix X1Àx Þ=N À x Á lTi ðhcp-bulkÞ f r À ð1 À xÞ Á lX ðbcc-bulkÞ ð1Þ2. Methods where N is the total number of atoms per supercell,2.1. Theoretical methods Er (TixX1Àx) is the total energy per supercell of the alloy, tot lTi/X is the chemical potential of element Ti or X in its cor- In order to identify Ti-based alloys which obey the con- responding bulk phase, respectively, and x is the alloy com-straints outlined in Section 1 (i.e. non-toxic elements, stable position. In the above deﬁnition (Eq. (1)) the alloy isin the b-phase, low Young’s modulus [1–30,34]) we have thermodynamically stable for Ef < 0.performed a systematic screening of binary alloys employ- In order to determine thermodynamic properties anding parameter-free density-functional theory calculations stability of phases at elevated temperatures, as, for exam-[31,32]. In this study, we restricted our research on Ti– ple, during the thermal treatment of the samples, theMo and Ti–Nb binaries, Mo and Nb both being non-toxic entropy eﬀects have to be considered. These can be decom-alloy ingredients. The aim of the calculations was to predict posed for solids into a conﬁgurational (mixing) and vibra-and understand metallurgical trends. In particular, we were tional contribution . In this study we use a roughinterested in a detailed understanding of how the alloy estimate of the temperature dependence and neglect thecomposition aﬀects the stability of the b-phase, and vibrational contribution which is computationally diﬃcultwhether and how it can be used to tailor the Young’s mod- to access. The remaining contribution, the conﬁgurationalulus. The calculations were performed using a plane wave entropy, is calculated in the ideal mixing approximation.pseudopotential approach as implemented in the Vienna This approximation becomes exact for alloys where the for-Ab initio Simulation Package (VASP) code [35,36]. The mation energy depends only on the concentration, not onplane wave cutoﬀ energy was 170 eV and a 8 · 8 · 8 Monk- the local atomic conﬁguration. As will be shown below,horst–Pack mesh was used to sample the Brillouin zone. the approximation is well justiﬁed in the case of the Ti-The binary alloys were described by supercells consisting alloys studied here. The ideal mixing entropy is given by:of 2 · 2 · 2 elementary cubic or hexagonal unit cells with S config ðxÞ ¼ k B Á ½x Á lnðxÞ þ ð1 À xÞ Á lnð1 À xÞ ð2Þa total of 16 atoms. A large variety of alloy compositionswere studied by systematically replacing Ti atoms by either where x is the alloy composition of a binary alloy TixX1ÀxNb or Mo atoms. The lowest alloy composition was and kB is the Boltzmann constant. The temperature depen-6.25 at.% (one Nb/Mo atom in a 16 atom supercell). For dent free energy can than be calculated according toeach alloy composition various local arrangements were F f ðx; T Þ ¼ hEf ðTix X1Àx Þi À T Á S config ð3Þconsidered, and in total 48 body-centered cubic (bcc) and28 hexagonal closed-packed (hcp) conﬁgurations were where the averaged formation energy ÆEf(TixX1Àx)æ is ob-studied. tained from the formation energies of alloys with diﬀerent For each of the constructed supercells the equilibrium local atomic conﬁguration but same concentration by aver-geometry was calculated, i.e. the geometry for which the aging using the Boltzmann statistics at the reference tem-total energy reaches a minimum and the forces on the perature. The temperature-dependent free energy ofatoms disappear and the system is strain free. Initially, formation allows to determine the thermodynamic stabilitywe performed a full relaxation both for the atoms (to of an alloy at a given temperature.reduce the forces acting on the atoms to zero) and forthe size and shape of the supercell (to make the system 2.2. Experimental methodsstrain-free). The biggest contribution turned out to bedue to the volume relaxation of the cubic supercell. Relax- The various Ti alloys were melted in an electric arc fur-ation eﬀects which are due to changes in the cell shape nace. All of the used alloy elements had a high purity(non-uniaxial components, shear components) or due to (Table 1). The electric arc furnace was evacuated and sub-displacements in the atomic positions were found to be sequently ﬂooded with argon at a pressure of 300 mbar.small with respect to the energy diﬀerences due to the vari- The furnace was equipped with a water-cooled copper cru-ations in the local arrangement. For the present study we cible. The temperature of the electric arc amounted totherefore neglected these relaxation eﬀects and took into about 3000 °C, while the melt was at the center hold at a
4478 D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487Table 1Alloy compositionsElement Ti20Mo7Zr5Ta Ti35Nb7Zr5Ta Ti10Nb Ti20Nb Ti25Nb Ti30Nb Ti10Mo Ti20Mo (wt.%) (wt.%) (at.%) (at.%) (at.%) (at.%) (at.%) (at.%) wt.% at.% wt.% at.% wt.% at.% wt.% at.% wt.% at.% wt.% at.% wt.% at.% wt.% at.%Ti 68 82.0 53 69.7 82.3 90 63.3 80 60.07 75 54.6 70 81.8 90 66.6 80Mo 20 12.0 18.2 10 33.4 20Zr 7 4.4 7 4.8Ta 5 1.6 5 1.7Nb 35 23.7 17.7 10 32.7 20 39.3 25 45.4 30peak temperature of 1830–1850 °C in order to assure com- received from this natural frequency into an electric currentplete dissolution of the Nb, Ta or Mo respectively. The of the same frequency and relative amplitude, during eightelectric arc method provided an intense stirring eﬀect. periods, due to a quartz clock where a reference crystalMelting all ingredients required about 30–60 s. oscillates at a given frequency. In order to obtain cast samples of optimal chemical and In order to determine the volume fractions of the twostructural homogeneity all specimens were remelted several phases after thermal homogenization experimentally, wetimes. This means that, after melting and stirring, each conducted X-ray wide angle diﬀraction experiments onsample was completely solidiﬁed in the crucible, then the various alloys. The measurements were conductedturned about its cross axis by use of an in-furnace manip- either with Mo Ka1 or Co Ka1 radiation obtained fromulator and subsequently reheated above the melting point. tubes operated at 40 mA and 40 kV. The crystallographicThis sequential procedure (melting, stirring, solidiﬁcation, textures of the cast and homogenized samples were weak,rotation) was repeated four times. After the fourth remelt- so that only a small corresponding error has to be takening step the sample was ﬁnally cast into a rectangular cop- into account.per mold of size 60 mm · 32.6 mm · 10 mm. The coppermold had a temperature of about 30 °C, which led to rapid 3. Results and discussionsolidiﬁcation, entailing only microsegregation and sup-pressing dendrite formation. 3.1. Thermodynamic analysis of phase stability: ab initio All as-cast samples were subjected to a solution heat simulationstreatment at 1473 K for 3 h in order to homogenize thesample and remove microsegregation. Since Ti alloys Based on Eq. (1), the T = 0 K formation energies for theundergo very strong chemical reactions with oxygen, the various ordered a and b structures have been calculatedsamples were generally heat treated under an argon atmo- (Fig. 1a and b). In order to analyze these data, we ﬁrstsphere. The more complex engineering alloy Ti–20 wt.% focus on the relative stability between the two phases.Mo–7 wt.% Zr–5 wt.% Ta was also solution annealed for According to Fig. 1a and b, both Nb and Mo destabilize3 h while the alloy Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta the a-phase (the formation energy increases with the com-was solution annealed for 4 h. position x) but stabilize the b-phase (the formation energy The ensuing characterization of the chemical and micro- decreases with composition x). Only for low concentrationsstructural homogeneity of the cast and heat-treated sam- of these elements (<10 at.% for Mo, <20 at.% for Nb) is theples was conducted by using optical and scanning a-phase found to be energetically more favorable than theelectron microscopy (SEM) in conjunction with energy dis- b-phase.persive X-ray spectrometry (EDX), electron backscatter Let us now focus on the thermodynamic stability. Fordiﬀraction (EBSD) and X-ray Bragg diﬀraction methods. an alloy to be thermodynamically stable its formation Grinding before microscopy was performed using 400, energy must be negative. According to Figs. 1a and b,600, 1200 and 2400 paper with subsequent use of 6 lm Nb and Mo exhibit a qualitatively diﬀerent behavior. For(45 min), 3 lm (20 min) and 1 lm (15 min) polishing. For Ti–Nb alloys the formation energies at temperatureoptical microscopy the samples were etched using a solu- T = 0 K of both the a- and b-phase are positive (endother-tion comprising 68 ml of glycerin, 16 ml of HNO3 and mic) for Nb concentrations up to 93 at.% (Fig. 1a). An16 ml of Hf. For SEM inspection, after the ﬁnal 1 lm pol- important implication of this result is that at low tempera-ishing step the specimens were ﬁnished by electrolytic pol- tures this alloy is thermodynamically completely immisci-ishing at 35 V for 60 s. ble in this concentration regime. Only for compositions The elastic properties were investigated by using an above 93 at.% the b-phase is intrinsically stable, i.e. theultrasonic resonance frequency method (Grindo-Sonic). alloy formation energy is negative (exothermic) even with-This method measures the elastic modulus by analyzing out any entropy stabilization eﬀects.the natural period of the transient vibration which results In contrast to the Ti–Nb system, for Ti–Mo alloys thefrom a mechanical disturbance of the object tested. The T = 0 K formation energy is endothermic only for lowGrindo-Sonic device transforms the incoming signal Mo concentrations but becomes exothermic at Mo concen-
D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487 4479Fig. 1. Theoretical alloy formation energies at T = 0 K (a and b) and free energies of formation at 1 K below the bcc–hcp transformation temperature inpure Ti, T = 881 °C (c and d) for binary Ti-X alloys as a function of the alloy composition. The images on the left hand side show the results for Ti–Nband those on the right hand side for Ti–Mo alloys. The (red) triangles/(blue) squares mark the formation energies for the hcp/bcc phase. The color of thebackground in (c) and (d) indicates the co-existing phases as calculated in Section 3.2: yellow: phase coexistence of hcp and bcc; blue: single-phase bcc. Thearrow shows the critical concentration x above which the bcc-phase becomes thermodynamically stable.trations larger than xcrit % 25 at.%. We therefore conclude lying the approximation of ideal mixing as used to derivethat Mo acts above a critical concentration xcrit as an Eq. (3) is well justiﬁed.intrinsic bcc stabilizer, i.e. it promotes the formation of A comparison of Fig. 1a and c shows that going fromthe bcc phase even in the absence of any entropy driven T = 0 K to ﬁnite temperatures signiﬁcantly reduces thetemperature eﬀects (Fig. 1a). alloy formation energy: while Nb stabilizes at T = 0 K In order to estimate the eﬀect temperature has on the the b-phase only at Nb concentrations well above 93%,formation/stabilization of the cubic phase, the alloy forma- ﬁnite temperature eﬀects strongly reduce the formationtion energy has been calculated at ﬁnite temperatures energy. As shown in Fig. 1c, close to the transformationemploying Eq. (3). A crucial issue is to deﬁne a suitable the- temperature the free energy of formation of b-Ti–Nb alloysoretical reference temperature to be used in Eq. (3). This becomes negative (exothermic) even for Nb concentrationsreference temperature can be regarded as a limit: below it as small as 25 at.%. We can therefore conclude that Nb actsthe system can no longer maintain thermodynamic equilib- as an entropy-driven b-stabilizer.rium and the phases which are thermodynamically stable at For Mo, which acts even at T = 0 K and in modest con-this temperature are frozen in rendering the system meta- centrations as a b-stabilizer (Fig. 1b), ﬁnite temperaturestable. At ﬁrst glance, it might be appealing to use the eﬀects are less pronounced (Fig. 1d): the minimum Moexperimental annealing temperature as a reference state. concentration at which the alloy formation energy becomesIn the annealing process the samples are kept for 3 h at this zero reduces from 25 to 14 at.%.temperature, which is suﬃcient for an alloy to reach ther- The fact that Mo is a better b-stabilizer then Nb is inmodynamic equilibrium. However, the annealing tempera- agreement with earlier experimental studies where Moture employed in our experiments (T = 1200 °C) is well was found to stabilize the b-phase already for Mo concen-above the transition temperature of Ti (T = 882 °C) and trations exceeding 5 at.% whereas 24 at.% of Nb was neces-the thermodynamic ground state of Ti is no longer hcp sary to achieve the same goal . A direct quantitativebut bcc. Therefore, we felt that a more suitable choice as comparison between our theoretical data and the experi-reference is the hcp–bcc transition temperature of Ti. The mental data in Refs. [38,39] is not straightforward. Thecorresponding results are shown in Fig. 1c and d. determination of the ﬁrst occurrence of a stable fraction According to Fig. 1a and b, the spread in energy for a of the b-phase by Dobromyslov and Elkin  was donegiven composition x but diﬀerent local conﬁgurations is by using an X-ray wide angle Bragg diﬀraction set-up insmall. This observation indicates that for the binary alloys conjunction with Cu Ka1 radiation. This method is preciseinvestigated the dependence of local conﬁguration on the usually only to a value of 1–3 vol.%. Also, the presence ofenergy of formation is weak. Thus, the assumption under- crystallographic textures may usually further reduce the
4480 D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487precision of the X-ray analysis for small amounts of a sec- alloy and 90 vol.% b-phase for the Ti–30 at.% Nbond phase. Also, Cu Ka1. radiation may create minor false alloy.intensity contributions such as those caused by For Ti–Nb alloys (Fig. 2c), the agreement betweenﬂuorescence. experiment and theoretical predictions is excellent. For Ti–Mo alloys, the agreement is less satisfactory. The dis-3.2. Thermodynamic analysis: comparison of the theoretical crepancy between theory and experiment may be due toresults and experimental data (i) neglecting vibrational entropy, which destabilizes the a-phase with increasing temperature; or (ii) the existence In order to address these issues, we experimentally deter- of another phase which has not been included in ourmined not only the onset of the b-phase but also its volume analysis.fractions for given alloy composition. An advantage of this An interesting conclusion can be drawn by inspectingapproach is that this quantity can be easily obtained from closer the Gibbs construction. According to Fig. 2b, thethe calculated formation energies by a Gibbs construction. Mo concentration in the a-phase should be close to zero. To actually perform the Gibbs construction, the compo- In order to verify this prediction, the phase content deter-sitional dependence of the averaged formation energy mined via X-ray diﬀraction was further cross-examined(Fig. 1c and d) was approximated by a third-order polyno- by joint EBSD and EDX measurements (see Fig. 4). A sig-mial using a least-squares approach. The Gibbs construc- niﬁcant diﬀerence between the Mo content in the a- and b-tions for both alloys and the computed volume fraction phases (Mo depleted in the latter) was indeed observed.of the b-phase are summarized in Fig. 2. The results were The EBSD images presented in Fig. 5 give an example ofalso used in Fig. 1c and d to determine the diﬀerent phase the experimentally observed microstructures for one of theregions (color-coding of the background). Employing the binary alloys, namely, for Ti–30 at.% Nb. Fig. 5a shows theGibbs construction, we ﬁnd that the threshold concentra- as-cast sample, while Fig. 5b shows the sample after chem-tions above which the alloys consist solely of the b-phase ical homogenization for 3 h at 1200 °C. One has to noteis $39 at.% of Nb and $36 at.% of Mo (Fig. 2). that the size bar is diﬀerent for the two micrographs owing In order to experimentally determine the volume to grain growth that took place during homogenizationfractions of the two phases after thermal homogenization, (Fig. 5b). The EBSD images reveal an isotropic grain shapewe conducted X-ray wide angle diﬀraction experiments for and a random texture in either case (before and afterthe binary Ti–Nb and Ti–Mo alloys (Fig. 3). The results, homogenization). The color code is the Miller index, aswhich are summarized in Table 2, are shown as ﬁlled green indicated in the standard triangle of lattice directionsstars in Fig. 2c and d. The experimental upper limits of the pointing in normal (i.e. casting) direction. The Kikuchiscreened alloys are 88 vol.% b-phase for the Ti–20 at.% Mo indexing procedure suggests that in the present case ofFig. 2. Gibbs construction (a and b) and volume fraction of the b-phase (c and d). Both binary alloy systems, Ti–Nb (a and c) and Ti–Mo (b and d), areshown. The volume fraction of the b-phase as determined by the ab initio method is shown by the (blue) dash-dotted line and empty blue stars for selectedconcentrations. The experimental data points (Table 2) are marked by ﬁlled green stars. The blue arrow marks the threshold concentrations for single-phase bcc alloys. The error bars for the experimental data fall within the symbol size.
D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487 4481Fig. 3. X-ray wide angle Bragg diﬀraction spectra for some of binary Ti–Nb and Ti–Mo alloys (Mo Ka1 radiation, 40 mA, 40 kV). The intensity is given inarbitrary units as a function of the diﬀraction angle 2h. (a) Binary Ti–Nb alloys; (b) binary Ti–Mo alloys.the Ti–30 at.% Nb alloy about 98% of all EBSD points 3.3. Ab initio predictions of the elastic properties in therevealed a bcc structure which is even larger than the value binary systems Ti–Nb and Ti–Moshown in Table 2 for the X-ray results. For samples withlower Nb content larger fractions of the a- and x-phase In order to identify metallurgical trends in the two bin-were found. ary alloy systems Ti–Nb and Ti–Mo with respect to the
4482 D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487Table 2Experimentally observed volume fractions of the phases based on the current measurements with Mo Ka1 radiationPhase content by X-ray Bragg diﬀraction Ti–10 at.% Nb Ti–20 at.% Nb Ti–25 at.% Nb Ti–30 at.% Nb Ti–10 at.% Mo Ti–20 at.% MoVolume fraction in %, a-phase (hcp) 94 40 19 10 26 12Volume fraction in %, b-phase (bcc) 6 60 81 90 74 88Fig. 4. EDX measurements in the two-phase microstructure of the Ti–10%Mo sample, which reveals close to zero intensity of Mo in the a-phase while theb-phase contains a high concentration of Mo. The sample was heat treated at 873 K for 4 days before the EDX measurement. desired mechanical properties (reduced stiﬀness), the Young’s modulus in the crystallographic [0 0 1] direction was calculated and analyzed for diﬀerent binary alloy com- positions. The theoretical predictions were based on the simulation of an uniaxial tensile test [40–42] along the crys- tallographic [0 0 1] direction of the b-phase. We proceeded in two steps. First, we determined the total energy of a given binary alloy in the ground state. In the second step, we applied an elongation along the [0 0 1] loading axis by a small ﬁxed amount e, which is a linear approximation (Hooke law) equivalent to the application of an elastic ten- sile stress r. For each value of the elongation e the total energy was minimized by relaxing two stresses in the direc- tions perpendicular to the loading axis. The stress r in the loading direction [0 0 1] is given by r ¼ ðdE=deÞ=ðA Á a0 Þ ð4Þ where E is the total energy per formula unit of the crystal, a0 is the ground state lattice parameter and A is the area (proportional to the formula unit of the crystal) perpendic- ular to the applied stress for each value of the elongation e.Fig. 5. EBSD images as an example of the experimentally observed The Young’s modulus is then deﬁned as the ratio betweenmicrostructures of one of the binary alloys, namely, of the Ti–30 at.% Nb the stress r and elongation e in the limit of a zero strainalloy. (a) The as cast sample; (b) the sample after homogenization for 3 h load. Applying this approach, the Young’s modules alongat 1200 °C. Note that the size bar is diﬀerent for the two micrographs the soft [0 0 1] direction have been calculated for both bin-owing to grain growth that took place during homogenization. The EBSDimages reveal an isotropic grain shape and a random texture. Color code: ary alloys (Fig. 6; blue squares). Also included in Fig. 6 areMiller index in standard triangle of lattice directions pointing in normal/ the experimental data points obtained from our ultrasoniccasting direction. measurements (green stars).
D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487 4483Fig. 6. Predicted and experimentally obtained Young’s moduli for two binary Ti alloy systems as a function of the alloy composition. (a) The results forthe Ti–Nb alloy; (b) the results for the Ti–Mo alloy. The blue squares show the simulation results for the soft [0 0 1] crystal direction of the bcc lattice cell.The green stars in both images represent experimental results obtained from our polycrystalline samples by ultrasonic measurements. The error bars fallwithin the symbol size. The experimental elastic modulus data were taken on samples which were cast and subsequently homogenized for 3 h at 1200 °C. The simulated data in Fig. 6 reveal that the Young’s sured moduli are 72.1 GPa for Ti–30 at.% Nb, 75.8 GPamodulus of the bcc Ti phase (b-phase) increases in both for Ti–20 at.% Nb and 91.2 GPa for Ti–10 at.% Nb, i.e.cases almost linearly with the alloy composition. The scat- the value observed for the Ti–30 at.% Nb alloy is the small-ter of the predicted modulus data stems from the variation est out of all the alloys which were experimentallyof the atomic conﬁguration in the cell, which was in all inspected. It must be noted that those materials with acases varied in order to evaluate the dependence of the small alloy content (10 at.%) most likely also contain sub-results on short range order eﬀects. It is interesting to note stantial amounts of the a- and x-phases, i.e. the stiﬀnessthat for the lowest alloy compositions (i.e. close to the limit data do not reﬂect the values of a pure bcc structure. Inof pure Ti) the Young’s modulus for the bcc phase becomes comparison, the bulk polycrystal modulus of the hexagonalnegative. A negative Young’s modulus implies that for low polycrystalline Ti sample which we measured as a referenceNb (<8 at.%) or Mo (<4 at.%) concentrations these bcc amounted to 114.7 GPa. This means that the best of thealloys are mechanically unstable against tetragonal elastic new binary materials, namely Ti–30 at.% Nb, yields a droploadings. This conclusion is in agreement with previous in stiﬀness of about 37%.studies on the elastic stability of bcc Ti (e.g. ), andreﬂects the fact that weakly alloyed Ti–Nb and Ti–Mo 3.4. Design of more complex engineering alloys on the basismaterials have the tendency to switch back into the stable of the theoretical predictionshexagonal phase when forced in the simulation into a bccstructure (Fig. 1). 3.4.1. Basic aspects The data points for the bulk polycrystal elastic data According to our novel strategy of a faster and moreshown in Fig. 6 in comparison to the predicted [0 0 1] elastic eﬃcient way for bottom-up alloy design as outlined in Sec-stiﬀness data have been taken from samples which have tion 1.2, we have in the second step of this work used thebefore been exposed to the 3 h, 1200 °C homogenization ab initio predictions obtained on the binary materialstreatment. These long heat treatments were done in order (Ti–Mo, Ti–Nb) as a starting point for the synthesis ofto approximate an thermodynamic equilibrium state in two more complex engineering alloy variants, namely,the samples and, thereby, to achieve better comparability Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta and Ti–20 wt.%with the theoretical predictions. Mo–7 wt.% Zr–5 wt.% Ta. In all cases, the experimentally determined Young’s To be more speciﬁc, in this discussion we properly iden-modulus is slightly larger than the theoretically estimated tify those aspects that were learned from the ab initio sim-results. The origin for this discrepancy is that the theoreti- ulations conducted on the two binary alloy systems withcal studies had been restricted to bulk single crystals while respect to more complex alloys design.the real samples are polycrystalline (see Fig. 5). In a poly- The ﬁrst points clearly demonstrated by the simulationscrystalline sample with random crystallographic texture the are the minimum threshold concentrations of the occur-Young’s modulus is isotropic and given by averaging the rence of a stable b-phase (together with a dominant a-Young’s moduli over a huge number of grains along all phase) and also of the stable single-phase existence of thecrystal orientations. The fact that averaging includes soft b-phase. The ﬁrst aspect is important when aiming at theand hard directions whereas the theoretical study focused design of a dual-phase alloy and the second one countson a single soft direction at T = 0 K may explain the dis- when aiming at a pure b-phase alloy with the smallest pos-crepancy between theory and experiment. sible elastic stiﬀness (because of the bcc structure). In that In the Ti–Mo system the experimentally observed mod- context, it was clearly observed from the simulationsuli for the new binary randomly oriented polycrystalline (matching experimental observations from the literaturealloys amount to 106.9 GPa for Ti–20 at.% Mo and and our own measurements) that Mo has a stronger eﬀect88.4 GPa for Ti–10 at.% Mo. In the Ti–Nb system the mea- on the formation of the b-phase than Nb. In other words,
4484 D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487Mo is a more eﬃcient bcc stabilizer in the Ti matrix than straints usually are contradictory since the resistance to dis-Nb. Another point pertaining to this aspect is the fact that, location motion and dislocation multiplication (strengthabove a critical concentration of about 25 at.%, Ti–Mo bcc and hardness) scales linearly with the magnitude of thealloys are intrinsically stable without the aid of the mixing shear modulus (in the isotropic limit of linear elasticity).entropy while Ti–Nb alloys are in general only entropy sta- A possibility to escape from this diﬃculty lies in a solidbilized. This means that the simulations clearly indicate the solution hardening strategy. This eﬀect is in any casediﬀerent thermodynamic quality for the two diﬀerent bcc already provided by the Nb or, respectively, Mo contentstabilizers. required for the basic stabilization of the bcc phase, and, This observation from the simulations is of great practi- for the case of more complex alloys, by minor addition(s)cal importance for engineering alloy design since Ti alloys of a second (or even second and third) bcc stabilizer (seeare typically in a strong non-equilibrium state when cast argumentation above), such as Ta and/or W, in solid solu-and, hence, require careful homogenization treatments. tion. Another element which could serve for solid solutionThis means that a more fundamental knowledge on the sta- hardening would be Zr. Further alloy alternatives are quitebility of diﬀerent alloy variants is very helpful in properly limited by the constraint of optimum biocompatibility.designing adequate heat treatments for alloy homogeniza-tion. Similar aspects apply to diﬀusion kinetics. 3.4.2. Application to engineering alloy design Another essential, though more practical, aspect of the Using the ab initio results in the spirit discussed abovethermodynamic insight into the stability of the alloys lies together with corresponding further alloy suggestions fromin choosing those alloying elements which stabilize the b- the literature [3–30], we designed, cast, processed and char-phase at the smallest possible alloy content, cost and/or acterized the two engineering alloy variants Ti–35 wt.%density increase. Nb–7 wt.% Zr–5 wt.% Ta and Ti–20 wt.% Mo–7 wt.% The second group of observations we used from the sim-ulations to design more complex materials along the linesprescribed by the two binary alloys is the evolution of theelastic modulus as a function of the alloying content. Theadvantage of predicting not only thermodynamic but alsomechanical data associated with our theory-guided alloydesign approach takes us beyond earlier conventional ther-modynamic approaches used before for alloy design, suchas that oﬀered by Calphad and similar methods. The ab ini-tio predictions of the elastic modulus clearly showed thatthe Ti–Nb bcc structure is less stiﬀ than the Ti–Mo bccstructure. This result reveals a conﬂict: on the one hand, the lowelastic modulus provided by a Ti–Nb-based bcc structureis highly desired for biomedical applications, but on theother hand, we found that this system is thermodynami-cally less stable. Hence, for more complex alloy design wecan learn that a Ti–Nb-based material should contain someadditional alloying content of another bcc stabilizer, suchas Ta, Mo or W. This strategy would most likely providea thermodynamically more stable bcc alloy with a smallelastic stiﬀness. Another essential feature associated with the bottom up-screening of the elastic properties is the possibility of pre-dicting and designing also the elastic anisotropy. Althoughthis aspect will be the subject of another publication, thepossibility for such a procedure is obviously at hand. Firsttests (which are not included in this work) have revealedthat not only the absolute values of the elastic propertiesbut also the anisotropy strongly changes as a function of Fig. 7. (a) EBSD images (normal plane indexed, data taken from threethe alloy content. This point can hence be exploited for fur- perpendicular directions) as an example of the experimentally observedther alloy design. microstructure of the as cast alloy Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta. (b) EBSD images (normal plane indexed, data taken from three A further point that can be learned form the binary alloy perpendicular directions) as an example of the experimentally observedpredictions with respect to more complex Ti-alloy design is microstructure of the as cast alloy Ti–20 wt.% Mo–7 wt.% Zr–5 wt.% Ta.the fact that the desire for a low elastic modulus should be ND, normal direction; RD, longitudinal direction; TD, transversecombined with high strength and hardness. These con- direction.
D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487 4485Zr–5 wt.% Ta. The EBSD maps in Fig. 7, taken for three clearly justify the use of ab initio simulations of the groundperpendicular sections, reveal that the texture of the cast state energy and of the temperature-dependent free energymaterial is practically random. for modern materials alloy design [44,45]. In both cases Both specimens revealed pronounced microsegregation (Ti–Nb, Ti–Mo) the basic tendency of the thermodynamicin the as-cast state which had to be removed by corre- stability and of the inﬂuence of the entropy have beensponding homogenization heat treatments at 1473 K properly predicted. Not only our own current experimental(1200 °C) under an argon atmosphere. The alloy Ti– results but also previous experimental observations20 wt.% Mo–7 wt.% Zr–5 wt.% Ta was solution annealed reported in the literature show that the tendency of Nbfor 3 h and the alloy Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% and Mo to form a stable bcc Ti alloy at higher alloy con-Ta was solution annealed for 4 h (Fig. 8). tent are correct. For the Ti–Nb binary alloy system it The X-ray spectra after heat treatment showed that the was also found that, although the Nb has the advantagematerial consisted essentially of the bcc phase. The volume of a strong reduction in its elastic modulus, it is not anfractions of the a- and x-phases were very small in both intrinsic stabilizer of the b-phase but requires the contribu-cases (Fig. 9). tion of the mixing entropy. According to the ab initio pre- While the bulk polycrystal modulus of the pure hexago- dictions for the Ti–Mo alloy system, the b-phase becomesnal Ti reference sample amounted to 114.7 GPa, that of the even intrinsically stable for Mo concentrations in the rangeheat-treated Ti–20 wt.% Mo–7 wt.% Zr–5 wt.% Ta alloy around 25 at.% without the contribution of any mixingwas 81.5 GPa and that of the heat-treated Ti–35 wt.% entropy. This means that, although the basic tendency ofNb–7 wt.% Zr–5 wt.% Ta alloy was as low as 59.9 GPa. high melting bcc refractory metals to stabilize the bcc phase of Ti has already been observed in the literature on the3.5. Discussion of the suitability of ab initio based design basis of empirical experience, the current ab initio simula-strategies in physical metallurgy tions have the clear advantage of revealing more clearly the true stability of the bcc phase created. Both the experimental results obtained for the binary An aspect which might deserve deeper future analysis inand those obtained for the engineering quaternary alloys the context of the free energy of Ti bcc phase is the possibleFig. 8. (a) EDX data before and after the heat treatment for the alloy Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta. (b) EDX data before and after the heattreatment for the alloy Ti–20 wt.% Mo–7 wt.% Zr–5 wt.% Ta.
4486 D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487Fig. 9. X-ray wide angle Bragg diﬀraction spectra of the two engineering alloys Ti–20 wt.% Mo–7 wt.% Zr–5 wt.% Ta and Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta after heat treatment (Co Ka1 radiation, 40 mA, 40 kV). The intensity is given in arbitrary units as function of the diﬀraction angle 2h.role of the vibrational entropy contribution in the stabiliza- ab initio simulations are very well suited for the bottom-tion of the b-phase. This may be relevant in the calculation up design of new alloys. Both the thermodynamic stabilityof the free energy, as known for some other bcc materials. and the elastic properties of the binary alloys could be pre-In the current paper we ignored this factor owing to the dicted well using ground state and free energy calculationsvery long and complex simulation procedures required to on the one hand and an ab initio elastic tensile test on thecover the point in depth. It will be addressed in a separate other.study. Beyond this clearly proven basic thermodynamic advan- Referencestage of the new method for modern alloy design, the pre-diction of the elastic stiﬀness by the ab initio tensile test  Brehme HJ. Titanium and titanium alloys, biomaterials of preference. Mem Etud Sci Rev Metall 1989:625.is of great relevance. It was shown, ﬁrst, that it is in prin-  de Gelas B, Molinier R, Seraphin L, Armand M, Tricot R. In:ciple possible to screen the elastic properties of new alloys Williams JC, Belov AF, editors. Titanium and titanium alloys. Newbefore actually melting and casting them, and secondly, York: Plenum Press; 1982. p. 2121.that the simulations are in good agreement with the exper-  Long MJ, Rack HJ. Biomaterials 1998;19:1621.imental observations.  Niinomi M. Metall Mater Trans A 2002;33A:477.  Wang K. Mater Sci Eng A 1996;213:134.  Niinomi M. Mater Sci Eng A 1998;243:231.4. Conclusions  Goldberg AJ, Burstone CJ. Dent Res 1979;58:593.  Burstone CJ, Goldberg AJ. Am J Orthod 1980;77:121. The study presented a new strategy for the theory-  Nelson KR, Burstone CJ, Goldberg AJ. Am J Orthod Dentofacialguided ab initio based bottom-up design of b-Ti alloys Orthop 1987;92:213.for biomedical applications using a quantum mechanical  Boyer RR, Rosenberg HW, editors. Beta titanium alloys in the 1980’s. New York: AIME; 1984. p. 209.approach in conjunction with experiments. The method  Lee CM, Ho WF, Ju CP, Chern Lin JH. J Mater Sci Mater Medwas applied to a set of binary Ti–Nb and Ti–Mo alloys. 2002;13:695.Following the predictions, the alloys were cast and charac-  Ho WF, Ju CP, Chern Lin JH. Biomaterials 1999;20:2115.terized with respect to their crystallographic structure,  Kuroda D, Niinomi M, Morinaga M, Kato Y, Yashiro T. Mater Sci Eng A 1998;243:244.microstructure, texture and elastic stiﬀness. In addition,  Niinomi M, Hattori T, Morkawa K, Kasuga T. Mater Transwe also studied two related engineering alloy compositions, 2002;43:2970.namely, Ti–35 wt.% Nb–7 wt.% Zr–5 wt.% Ta and Ti–  Niinomi M. Biomaterials 2003;24:2673.20 wt.% Mo–7 wt.% Zr–5 wt.% Ta. The results show that  Ankem S, Greene CA. Mater Sci Eng A 1999;263:127.
D. Raabe et al. / Acta Materialia 55 (2007) 4475–4487 4487 Prima F, Vermaut P, Ansel D, Debuigne J. Mater Trans 2000;41:  Li SJ, Yang R, Li S, Hao YL, Cui YY, Niinomi M, et al. Wear 1092. 2004;257:869. Weiss I, Semiatin SL. Mater Sci Eng A 1998;243:46.  Hohenberg P, Kohn W. Phys Rev 1964;136:B864. Ikeda M, Komatsu S-Y, Sowa I, Niimoni M. Metall Mater Trans  Kohn W, Sham LJ. Phys Rev 1965;140:A1133. 2002;33A:487.  Perdew JP, Burke K, Ernzerhof M. Phys Rev Lett 1996;77: Geetha M, Singh AK, Muraleedharan K, Gogia AK. J Alloys Compd 3865. 2001;329:264.  Hanada S, Matsumoto H, Watanabe S. In: International congress Hao YL, Niimoni M, Kuroda D, Fukunaga K, Zhou YL, Yang R, series, vol. 1284; 2005. p. 239. et al. Metall Mater Trans A 2003;34A:1007.  Kresse G, Hafner J. Phys Rev B 1993;47:558. Banerjee R, Nag S, Fraser HL. Mater Sci Eng C 2005;25:282.  Kresse G, Furthmuller J. Phys Rev B 1996;54:11169. ¨ Nag S, Banerjee R, Fraser HL. Mater Sci Eng C 2005;25:357. ´  Turchi PEA, Drchal V, Kudrnovsky J, Colinet C, Kaufman L, Liu Z- Banerjee R, Collins PC, Bhattacharyya D, Banerjee S, Fraser HL. K. Phys Rev B 2005;71:094206. Acta Mater 2003;51:3277.  Zhang Y, Liu H, Jin Z. Calphad 2001;25:305. Banerjee R, Nag S, Stechschulte J, Fraser HL. Biomaterials  Dobromyslov AV, Elkin VA. Scripta Mater 2001;44:905. 2005;25:3413.  Price DL, Cooper BR, Wills JM. Phys Rev B 1992;46:11368. Prima F, Debuigne J, Boliveau M, Ansel D. J Mater Sci Lett ˇ  Sob M, Wang LG, Vitek V. Mater Sci Eng A 1997;234–236:1075. 2000;19:2219. ´ ˇ  Friak M, Sob M, Vitek V. Phys Rev B 2003;68:184101. Aziz-Kerrzo M, Conroy KG, Fenelon AM, Farrell ST, Breslin CB. ˇ  Wang LG, Sob M, Zhang Z. J Phys Chem Sol 2003;64:863. Biomaterials 2001;22:1531.  Ikehata H, Nagasako N, Kuramoto S, Saito T. MRS Bull 2006;31: Yu SY, Scully JR. Corrosion 1996;53:965. 688. Godley R, Starosvetsky D, Gotman I. J Mater Sci – Mater Med  Ikehata H, Nagasako N, Furuta T, Fukumoto A, Miwa K, Saito T. 2006;17:63. Phys Rev B 2004;70:174113.